Room F14, Renold Building University of Manchester 2325 June 2010
Please note: abstract books will NOT be distributed at the workshop. If you would like to bring a copy of the book to the workshop you should download a copy from here and print your own.
Sponsors:
(IoP Nanoscale Physics and Technology Group (link opens in a new window)) (IoP Quantum Electronics and Photonics Group) (IoP Computational Physics Group)
(Computational Science & Engineering Department)
Organisers:
Stanko Tomic (STFC Daresbury Laboratory) Eoin O'Reilly (Tyndall National Institute) Max Migliorato (University of Manchester) G.P.Srivastava (University of Exeter)
This three day workshop will take place at the University of Manchester from 2325 June and will follow on from a similar workshop to be held at the Tyndall Instutute in Dublin on 21 and 22 June. The Dublin meeting will focus on the more technical aspects of the subject with this Manchester workshop concentrating on the science aspect. A more detailed description of the subject for this workshop is included for information below.
Registration
If you would like to attend this workshop please complete the ONLINE REGISTRATION FORM. The workshop has a limit of 50 places and the registration form will be disabled once this limit is reached.
Two registration fees will be in operation for this event...
Academic Delegates Ã¯Â¿Â½35 NonAcademic Delegates Ã¯Â¿Â½70
Details of how to pay your registration fees can be found here.
[NOTE: by completing this form you are only registering for the Manchester workshop. If you would also like to register for the workshop in Dublin then you must visit the Dublin workshop web pages]
Speakers and Participants
Speakers and participants confirmed so far include...
Pawel Hawrylak (Institute for Microstructural Sciences, Canada) XiangWei Jiang (Institute of Semiconductor, Chinese Academy of Science, China) Guy Allan (Institut d'Electronique, de Micoelectronique et de Nanotchnology, France) Frederic Aniel (University of Paris, France) Urs Aeberhard (IEF5 Photovoltaik Forschungszentrum JÃ¯Â¿Â½lich, Germany) Gabriel Bester (MaxPlanckInstitut fur Festkorperforschung, Germany) Stefan Birner (nextnano3, Germany) Andrei Schliwa (KonradZuseZentrum fÃ¯Â¿Â½r Informationstechnik Berlin, Germany) Bernd Witzigmann (University of Kassel, Germany) Brad Foreman (Hong Kong University of Science and Technology, Hong Kong) Aldo Di Carlo (University of Rome "Tor Vergata", Italy) Guido Goldoni (INFMCNR S3 and University of Modena and Reggio Emilia, Italy) Wlodek Zawadzki (Polish Academy of Sciences, Poland) Mikhail Nestoklon (IOFFE Institute, Russia) Nikola Prodanovic (University of Belgrade, Serbia and Montenegro) Juan Manuel Llorens Montolio (Insitute of Microelectronics of Madrid, CSIC, Spain) Christof Voemel (ETH Zurich, Switzerland) David Binks (University of Manchester, UK) Marco Califano (University of Leeds, UK) Ned EkinsDaukes (Imperial College London, UK) Andy Sunderland (STFC Daresbury Laboratory, UK) Timothy Boykin (University of Alabama at Huntsville, USA) Thomas Chanier (University of Iowa, USA) Michael Flatte (University of Iowa, USA) Lok Lew Yan Voon (Wright State University, USA) LinWang Wang (Lawrence Berkely National Laboratory, USA) Vladimir Falko (University of Lancaster, UK)
Programme
The timetable for the workshop will be added here as speakers are confirmed but we aim to start with registration from 08:00  10:00 on Wednesday 23 June. The workshop will close at 16:00 on Friday 25 June.
Proceedings
The proceedings from this meeting will be published in the open access Journal of Physics: Conference Series, which is published by IOP Publishing. Details of how to submit a paper plus information on formatting can be found here.
Accommodation
If you require accommodation for the duration of the workshop then you must make your own arrangements.
You can find information about hotels in Manchester from the following web pages... www.Otel.com/ManchesterHotels www.booking.com/Manchester www.directhotels.co.uk/citymanchester.htm
Travel to Manchester
Information on travelling to Manchester will be provided soon. Please check back regularly.
Detailed Workshop Description
Theory, modelling, and computational methods for semiconductor materials and nanostructures is a topic of rapid growth and great international interest. A lot of the worldwide effort over the past 50 years in establishing the theoretical foundation of methodologies for calculations of structural, electronic, optical and transport (electrical and thermal) properties of semiconductor nanostructured materials [161] are now coming to fruition [6267].
Modern crystalgrowth techniques, such as molecular beam epitaxy or metalorganic chemicalvapour deposition, are capable of producing prescribed crystal structures, sometimes even in defiance of equilibrium bulk thermodynamics.
To correlate desired electronic and optical properties with the structure cannot be efficiently done experimentally solely by trialanderror methods. Hence computational methods and novel algoritms that combine fast empirical solvers, detailed knowledge of the nanostructure shape and size, chemical composition, and mechanical properties, together with ever increasing computational power available are required to address this fundamental problem.
Among the many empirical methods available, the multiband k.p (k.p), empirical tight binding (ETB), and empirical pseudopotential (EPM) methods are proving invaluable in the design and modelling of modern optoelectronic devices and semiconductor nanostructures.
After the pioneering work on electronic structure of Luttinger and Kohn [1] and Kane [2,5] on the perturbative approach, the k.p method, for electronic structure of bulk and strained material in the vicinity of the characteristic points in the Brillouin zone (usually the Gamma point), with only a limited number of states in the expansion, now days the implementation of the k.p Hamiltonian constantly evolves and now encompasses 16 [12], 24 or even 30 [28] [28a]. The latest development of the k.p theory, using accurate parameterizations obtained from many body perturbation theory in the GW approximation, are capable of describing the electronic structure of the whole Brillouin zone of IIIV materials [p4]. Recent efforts on parameterization of the k.p Hamiltonian, for wurtzite structures also include the use of DFT calculation with optimised effective potentials (OEP) [p5]. The most commonly used implementation of the k.p Hamiltonian now days is the 8band k.p Hamiltonian, which takes into account mixing of the valence band states between themselves, mixing of the lowest conduction band state with few top valence band states, and also takes into account the effect of the spinorbit interaction [31]. The Spin orbit effect, although regularly ignored in firstprinciples calculations, is crucial in low energy gap materials like InAs or InSb [5], and in alloys with heavy atoms, like lead containing binaries PbSe etc [29]. The wide use of the 8band k.p method also owes to the transferability of the Hamiltonian over the whole family of the IIIV materials [p6]. With new computer architecture the 8band k.p Hamiltonian is now regularly used for calculation of the electronic structure of semiconductor nanostructures: quantum dots, quantum dashes, quantum wires, etc [18,19,21,22,24,25,33,37,n1,n4,n5]. The flexibility of the 8band k.p model also allows for relatively easy rotation of the kinetic, strain and piezoelectric part of the Hamiltonian to allow research of nanostructures grown on high Miller index planes [15,33]. In the plane waves implementation, the multiband k.p code for QD structure, was recently successfully used to relate absorption characteristics and optimal QD arrangements in Intermediate Band Solar Cells (IBSC) based on QD arrays [37]
The development of atomistic empirical potential methods for Molecular Dynamics (MD) and Molecular Statics (MS) has allowed structural simulations of low dimensional IIIV semiconductor materials to become a field that has attracted a substantial amount of interest in recent years [3847] There are several reasons for this, the most important probably being that the electronic properties of lattice mismatched epitaxial semiconductor layers are strongly affected by their structural properties [48]. Hence the reliable determination of quantities such as the elastic properties and the resulting strain is a fundamental prerequisite for implementing any accurate description of the bandstructure and the associated energy levels [49].
The stateoftheart at present is represented by the well known AbelTersoff potentials (ATPs) [5055], Stillinger Weber potential, [56] and the KeatingValence Force Field [4] method. Despite their wide use some fundamental questions need to be resolved, particularly in the inefficiency and inaccuracy of these potentials in describing the phonon spectrum [58]. Current attempts at solving these problems concentrate on superimposing the essence of the pbonding to the sbonding in order to capture more of the physical and chemical behaviour [59]. This however might create an extremely computational intensive problem if the potential is to be used within large MD problems. Hence specialized approaches to parallelization of these routines are extremely timely.
Of the empirical approaches to calculate the bandstructure of semiconductor materials Tight Binding (TB) has for a long time been regarded as a very accurate but not ideal alternative to k.p and empirical pseudopotential method (EPM), mainly because of the computational demand. The TB approach is in origin an approximated ab initio technique that relies on constructing the band structure from a truncated linear combination of atomic orbitals (LCAO). However it was proposed that the method could also be used as a semi empirical approach when the Hamiltonian matrix elements in the basis of the atomic orbitals are used as fitting parameters. This opened the way for the Empirical Tight Binding (ETB) approach which is generally found in two Ã¯Â¿Â½flavoursÃ¯Â¿Â½ for applications to semiconductor nanostructures: either using the sp3s* valence shells and interactions up to second nearest neighbours, or the sp3d5s* ones and only nearest neighbour interactions. The s* is a virtual orbital, that can be viewed as an excited s orbital, introduced by Vogl et al, [10] to mimic, in nearest neighbour models, the effect of the higher momentum orbitals.
While both ETB and EPM reduce the need for fitting in the final results by obtaining accurate parameterisations from the bulk and strained crystal properties, the main advantages of using ETB for calculating the electronic levels of nanostructures is that the treatment of the strain induced deviations from the bulk band structure is nearly self consistent: unlike the screened EPMs which depend explicitly on the strain (even if it is only the hydrostatic strain), the ETB parameters scale with increasing bond length (this feature is known as HarrisonÃ¯Â¿Â½s scaling rule) to take into account the hydrostatic strain, while the formulation itself has a strong dependence on the bond angle (through the Bloch phases [exp (i k.r)] between different nearest neighbour atoms, which clearly takes care of the effects of the shear strain. Furthermore as an atomistic method it is also possible to treat problems like piezoelectricity self consistently, even though a solution to the problem has not yet been clearly identified.
There is no doubt that despite parameterisations being available for all commonly used semiconductors,[60] ETB applied to semiconductor nanostructures still requires significant computational power. In general the use of the sp3d5s* (20 orbitals) approach for N atoms requires the solution of a 20xN order matrix, utilising 22 parameterised two centre integrals,[61,n3] hence the need for parallel clusters machines.
The stateoftheart tight binding calculations were recently used to investigate influence of electronic structure and multiexciton spectral density on multipleexciton generation in semiconductor nanocrystals (Si, InAs, PbS) and its possible application in photovoltaic device [36].
The essence of the Empirical Pseudopotential Method (EPM) is to provide nonself consistent band structure calculations for crystals and nanocrystals with a full and accurate description of both occupied and unoccupied states over a large energy range. This is usually achieved by Ã¯Â¿Â½fittingÃ¯Â¿Â½ the pseudopotential (i.e. potential experienced by chemically active electrons in their valence shell) in momentum (or reciprocal) space. Due to crystal symmetry, this requires only fitting the Fourier components v(G) of the pseudopotential corresponding to only a few shortest reciprocal lattice vectors {G}. For solids with super structures, or for nanocrystals, v(G) corresponding to shorter G vectors can be interpolated from the values for the relevant bulk materials. The earliest successful application of the EPM was made for explaining optical measurement on semiconductors by Cohen and Bergstresser [3] who employed the socalled local EPM and by Chelikowsky and Cohen [9] who employed the socalled nonlocal EPM, including spinorbit interaction. More recent successful applications of the EPM for superlattices and nanostructures have been made by several groups [13,20,23,26,p1,n2,n7]. As the EPM method is nonself consistent it is computationally much cheaper and faster to apply than abinito methods. Moreover, as it deals with both occupied and unoccupied states on equal footing, it is very useful for studying optoelectronic properties without requiring any further adjustment to the theory of band structure.
Further development of the EPM, particularly desirable for electronic structure calculations of quantum dots includes the linear combination of bulk bands (LCBB) variant of the full EPM [20]. In the LCBB method the wave functions of a nanostructure (superlattice, wire, and dot) are expanded as linear combinations of a limited number (n) of the bulk Bloch states of the constituent materials and wave vectors k. This flexibility allows one to use physical intuition in selecting the n and k that are most relevant for a given problem.
The EPM method was successfully used to predict excitonic properties of the novel solar cells based on multi exciton generation (MEG) mechanisms in CdSe QDÃ¯Â¿Â½s and role of Auger processes in MGE [26]
Stateofthe art application of the EPM method as a fast empirical [20,n7] solver in combination with stochastic search engines allows determination of the crystal structure with preassigned electronic and optical properties [63]. To correlate desired electronic and optical properties with the structure cannot be efficiently done solely experimentally by trialanderror methods. Hence the computational solution of the inverse problem address the fundamental problem of finding the atomic configuration of a complex, multicomponent system that produces a target electronicstructure property.
Electronic structure methods, such as multiband k.p, Empirical Tight Binding and Empirical Pseudopotential, coupled with empirical methods for the determination of the crystal structure (Valence Force Field, Bond Order Potentials) have recently seen much improvement in both the methodology, parameterizations and computational speed. The next step will certainly be that of condensing and interfacing all the individual efforts to produce tools that are of more general use to the wider community. It is therefore now very timely to devote two closely coupled CECAM Workshops to the use of empirical methods for semiconductor nanostructure design and modelling, with the first (ACAM) Workshop focused primarily on computational/technical issues, numerical implementations and parametrisation strategies, followed immediately by the second (STFC Daresbury) Workshop highlighting the scientific issues and demands related to empirical nanostructure design and modelling.
References
a) General Reference
[1] J. M. Luttinger and W. Kohn, "Motion of Electrons and Holes in Perturbed Periodic Fields", Phys. Rev. 97, 869 (1955).
[2] E. O. Kane, "Band Structure of Indium Antimonide", J. Phys. Chem. Solids 1, 249 (1957).
[3] M. L. Cohen and T. K. Bergstresser, Phys. Rev. 141, 789 (1966).
[4] P. N. Keating, "Effect of Invariance Requirements on the Elastic Strain Energy of Crystals with Application to the Diamond Structure", Phys. Rev. 145, 637 (1966).
[5] E.O. Kane, "The kp method", Semiconductors and Semimetals (New York: Academic) p.75 (1967)
[6] V. Heine, "The concept of Pseudopotentials" Solid State Physics 24, 1 (1970).
[7] R. M. Martin, "Elastic Properties of ZnS Structure Semiconductors", Phys. Rev. B 1, 4005 (1970).
[8] A. Baldereschi, "MeanValue Point in the Brillouin Zone", Phys. Rev. B 7, 5212 (1973)
[9] J. R. Chelikowsky and M. L. Cohen, "Nonlocal pseudopotential calculations for the electronic structure of eleven diamond and zincblende semiconductors", Phys. Rev. B 14, 556 (1976)
[10] P. Vogl, H. P. Hjalmarson and J.D. Dow, "A Semiempirical tightbinding theory of the electronic structure of semiconductors", J. Phys. Chem. Solids 44, 365 (1983)
[11] J. Robertson, E. P. OÃ¯Â¿Â½Reilly "Electronic and atomic structure of amorphous carbon," Phys. Rev. B 35, 2946  2957 (1987)
[12] M. Cardona, N. E. Christensen, and G. Fasol, "Relativistic band structure and spinorbit splitting of zincblendetype semiconductors", Phys. Rev. B 38, 1806 (1988)
[13] P. Friedel, M. S. Hybertson and M. SchlÃ¯Â¿Â½ter, Phys. Rev. B 39, 7974 (1989).
[14] Al. L. Efros, "Luminescence polarization of CdSe microcrystals," Phys. Rev. B 46, 7448 (1992)
[15] ShuShen Li and JianBai Xia, "Effectivemass theory for GaAs/Ga1xAlxAs quantum wires and corrugated superlattices grown on (311)oriented substrates", Phys. Rev. B 50, 8602 (1994)
[16] Al. L. Efros and M. Rosen, "Random Telegraph Signal in the Photoluminescence Intensity of a Single Quantum Dot", Phys. Rev. Lett. 78, 1110  1113 (1997)
[17] B. A. Foreman, "Analytical EnvelopeFunction Theory of Interface Band Mixing", Phys. Rev. Lett. 81, 425 (1998)
[18] C. Pryor, Eightband calculations of strained InAs/GaAs quantum dots compared with one, four, and sixband approximations, Phys. Rev. B 57, 7190 (1998)
[19] C.Pryor, J. Kim, L. W. Wang, A. J. Williamson, and A. Zunger, "Comparison of two methods for describing the strain profiles in quantum dots," J. Appl. Phys. 83, 2548 (1998)
[20] L.W. Wang, A. Zunger, "Linear combination of bulk bands method for large scale electronic structure calculations on strained nanostructures", Phys. Rev. B 59, 15806 (1999).
[21] O. Stier, M. Grundmann, and D. Bimberg , "Electronic and optical properties of strained quantum dots modeled by 8band kp theory", Phys. Rev. B 59, 5688 (1999)
[22] A.D. Andreev and E.P. OÃ¯Â¿Â½Reilly, "Theory of the electronic structure of GaN/AIN hexagonal quantum dots," Phys. Rev. B 62, 15851, (2000)
[23] A. J. Williamson, L.W. Wang and A. Zunger, Phys. Rev. B 62, 12963 (2000).
[24] W. Sheng and J.P. Leburton, "Anomalous QuantumConfined Stark Effects in Stacked InAs/GaAs SelfAssembled Quantum Dots", Phys. Rev. Lett. 88, 167401 (2002)
[25] S. Sauvage P. Boucaud R. P. S. M. Lobo, F. Bras, G. Fishman R. Prazeres, F. Glotin, J. M. Ortega, J.M. GÃ¯Â¿Â½rard, "Long Polaron Lifetime in InAs/GaAs SelfAssembled Quantum Dots", Phys. Rev. Lett. 88, 177402 (2002)
[26] LW. Wang, M. Califano, A. Zunger, A. Franceschetti, "Pseudopotential Theory of Auger Processes in CdSe Quantum Dots," Phys. Rev. Lett. 91, 056404 (2003)
[27] V. Ranjan, G. Allan, C. Priester, et al., "Selfconsistent calculations of the optical properties of GaN quantum dots" Phys. Rev. B 68, 115305 (2003)
[28] S. Richard, F. Aniel, and G. Fishman, "Energyband structure of Ge, Si, and GaAs: A thirtyband kp method", Phys. Rev. B 70, 235204 (2004)
[28a] Lok C. Lew Yan Voon and M. Willatzen, "The kp MethodElectronic Properties of Semiconductors," (Springer, Berlin 2009)
[29] G. Allan and C. Delerue, "Confinement effects in PbSe quantum wells and nanocrystals" Phys. Rev. B 70, 245321 (2004)
[30] M.A. Migliorato, D. Powell, A.G. Cullis, T. Hammerschmidt and G.P. Srivastava, "Composition and strain dependence of the piezoelectric coefficients in InxGa1xAs alloys", Phys. Rev. B 74, 245332 (2006)
[31] W. Zawadzki and P. Pfeffer, "Spin splitting of subband energies due to inversion asymmetry in semiconductor heterostructures", Semicond. Sci. Technol. 19, R1 (2004)
[32] B. Partoens and F.M. Peeters "From graphene to graphite: Electronic structure around the K point", Phys. Rev. B 74, 075404 (2006)
[33] V. Mlinar and F. M. Peeters, "Optical properties of (In,Ga)As capped InAs quantum dots grown on [11k] substrates", Appl. Phys. Lett. 91, 021910 (2007).
[34] D. Powell, M.A. Migliorato and A.G. Cullis, "Optimised Tersoff Potential Parameters for tetrahedrally bonded IIIV semiconductors", Phys. Rev. B 75, 115202 (2007)
[35] B. A. Gillespie, X. W. Zhou, D. A. Murdick, H. N. G. Wadley, R. Drautz, and D. G. Pettifor, "Bondorder potential for silicon," Phys. Rev B 75, 155207 (2007)
[36] G. Allan and C. Delerue, "Influence of electronic structure and multiexciton spectral density on multipleexciton generation in semiconductor nanocrystals: Tightbinding calculations," PHYSICAL REVIEW B 77, 125340 (2008)
[37] S. Tomic, T.S. Jones, and N.M. Harrison, "Absorption Characteristics of a Quantum Dot Array Induced Intermediate Band: Implications for Solar Cell Design," Applied Physics Letters 93, 263105 (2008)
[38] R. Smith 1992 Nucl. Instr. Meth. Phys. Res. B 67, 335 (1992)
[39]M. Sayed, J.H. Jefferson, A.B. Walker and A.G. Cullis, Nucl. Instr. Meth. Phys. Res. B 102, 218 (1995)
[40] P.A. Ashu, J.H. Jefferson, A.G. Cullis, W.E. Hagston and C.R. Whitehouse, J. Crystal Growth 150, 176 (1995)
[41] M. Nakamura, H. Fujioka, K. Ono, M. Takeuchi, T. Mitsui and M. Oshima, J. Crystal Growth 209, 232 (2000)
[42] F. Benkabou, H. Aourag, P..J. Becker and M. Certier, Mol. Sim. 23, 327 (2000)
[43] M.A. Migliorato, A.G. Cullis, M. Fearn and J.H. Jefferson, Phys. Rev. B 65, 115316 (2002)
[44] W.H. Moon and H.J. Hwang, Phys. Lett. A 315, 319 (2003)
[45] S. GoumriSaid, M.B. Kanoun, A.E. Merad, G. Merad and H. Aourag, Chem. Phys. 302, 135
[46] S.R. Billeter, A. Curioni, D. Fischer, W. Andreoni, Phys. Rev. B 73, 155329 (2006)
[47]R. Drautz , D.A. Murdick, D. NguyenManh, X.W. Zhou, H.N.G. Wadley, D.G. Pettifor, Phys. Rev. B 72, 144105 (2005)
[48] F.H. Pollak, Semiconductors and Semimetals 32, 17 (1990)
[49]J. Singh, Physics of Semiconductors and their Heterostructures (McGraw Hill) (1993)
[50] G.C. Abell, Phys. Rev. B 31, 6184 (1985)
[51] J. Tersoff, Phys. Rev. Lett. 56, 632 (1986)
[52] J.Tersoff, Phys. Rev. B 37, 6991 (1988)
[53] J.Tersoff, Phys. Rev. B 39, 5566 (1989)
[54] D. Conrad and K. Scheerschmidt, Phys. Rev. B 58, 4538 (1998)
[55] D. Powell, M. A. Migliorato, and A. G. Cullis, Phys. Rev. B 75, 115202 (2007)
[56] F.H. Stillinger and T.A. Weber, Phys. Rev. B 31, 5262 (1985)
[57] P.N. Keating, Phys. 145, 637, ibid 149, 674 (1966)
[58] L.J. Porter, S. Yip, M. Yamaguchi, H. Kaburakai and M. Tang, J. Appl. Phys. 81, 96 (1997)
[59] B. A. Gillespie, X. W. Zhou, D. A. Murdick, H. N. G. Wadley, R. Drautz, and D. G. Pettifor, Phys. Rev. B 75, 155207 (2007)
[60] S Turcotte, N Shtinkov , P Desjardins, RA Masut, R Leonelli, J. Vac. Sci. Technol. A 22, 776 (2004)
[61] TB Boykin, G Klimeck, RC Bowen, F Oyafuso, Phys Rev B 66, 125207 (2002)
[62] A. K. Geim, I. V. Grigorieva, S. V. Dubonos, J. G. S. Lok, J. C. Maan, A. E. Filippov & F. M. Peeters, "Phase transitions in individual submicrometre superconductors",Nature 390, 259 (1997)
[63] A. Franceschetti and A. Zunger, "The inverse handstructure problem of finding an atomic configuration with given electronic properties", Nature 402, 60 (1999).
[64] M. Bayer, O. Stern, P. Hawrylak, S. Fafard & A. Forchel, "Hidden symmetries in the energy levels of excitonic 'artificial atoms", Nature 405, 923(2000)
[65] M. Bayer, P. Hawrylak, K. Hinzer, S. Fafard, M. Korkusinski, Z. R. Wasilewski, O. Stern, A. Forchel, "Coupling and Entangling of Quantum States in Quantum Dot Molecules", Science 291, 451 (2001)
[66] D. Kitchen, A. Richardella, J.M. Tang, M. E. Flatte and A. Yazdani, "Atombyatom substitution of Mn in GaAs and visualization of their holemediated interactions", Nature 442, 436 (2006)
[67] S. Kalliakos, M. Rontani, V. Pellegrini, C.P. Garcia, A.Pinczuk, G. Goldoni, E. Molinari, L.N. Pfeiffer, and K.W. West, "A molecular state of correlated electrons in a quantum dot", Nature Physics 4, 467 (2008)
b) Parametrization:
[p1] L.W. Wang and A. Zunger, "Pseudopotentialbased multiband k.p method for 250 000atom nanostructure systems", Phys. Rev. B 54, 11417, (1996)
[p2] Y.M. Niquet YM, C. Delerue, and G. Allan, et al., "Method for tightbinding parametrization: Application to silicon nanostructures", Phys. Rev. B 62, 5109 (2000)
[p3] G. Bester, X. Wu, D. Vanderbilt, and A. Zunger, Phys. Rev. Lett. 96, 187602 (2006).
[p4] D. Rideau, M. Feraille, L. Ciampolini, M. Minondo, C. Tavernier, and H. Jaouen, and A. Ghetti, "Strained Si, Ge, and SiGe alloys modelled with a firstprinciplesoptimized fullzone k.p method", Phys. Rev. B 74, 195208 (2006)
[p5] P. Rinke, M. Winkelnkemper, A. Qteish, D. Bimberg, J. Neugebauer, and M. Scheffler, Phys. Rev. B 77, 075202 (2008).
[p6] I. Vurgaftman, J.R. Meyer, and L.R. RamMohan, "Band parameters for IIIV compound semiconductors and their alloys", J. Appl. Phys. 89, 5815, (2001)
c) Numerical implementation:
[n1] O. Stier, Electronic and Optical Properties of Quantum Dots and Wires (Wissenschaft & Technik Verlag, Berlin, 2000).
[n2] A. Canning L. W. Wang, A. Williamson and A. Zunger, "Parallel Empirical Pseudopotential Electronic Structure Calculations for Million Atom Systems", J. Comp. Phys. 160, 29 (2000)
[n3] G. Klimeck, F. Oyafuso, T. B. Boykin, R. C. Bowen, and P. von Allmen, "Development of a Nanoelectronic 3D (NEMO 3D) Simulator for Multimillion Atom Simulations and Its Application to Alloyed Quantum Dots", Computer Modelling in Engineering and Science (CMES) Volume 3, No. 5 pp 601642 (2002).
[n4] S. Tomic, A.G. Sunderland, and I.J. Bush, "Parallel multiband kp code for electronic structure of zincblend semiconductor quantum dots," Journal of Materials Chemistry 16, 1963 (2006)
[n5] S. Birner, T. Zibold, T. Andlauer, T. Kubis, M. Sabathil, A. Trellakis, P. Vogl, "nextnano: General Purpose 3D Simulations" IEEE Transactions on Electron Devices 54 (9), 2137 (2007)
[n6] C. Vomel, S. Z. Tomov, O. A. Marques, A. Canning, L.W. Wang and J. J. Dongarra, "Stateoftheart eigensolvers for electronic structure calculations of large scale nanosystems", J. Comp. Phys. 227, 7113 (2008)
[n7] G. Bester, "Electronic excitations in nanostructures: An empirical pseudopotential based approach," J. Phys. Cond. Mat. .21, 023202 (2009)
